Microscale investigation of arsenic distribution and species in cement product from cement kiln coprocessing wastes.
In many developing countries, the use of cement kilns to coprocess wastes containing heavy metals is thriving and plays an exceedingly important role in solid waste, especially hazardous waste disposal [1-3]. Coprocessed wastes include electroplating sludge, contaminated soil, chromium slag, sludge, hazardous combustible liquid wastes, and garbage . During coprocessing, almost all nonvolatile and semivolatile heavy metals are transferred into cement clinker which causes the heavy metal concentration in the cement to increase significantly. These heavy metals in cement will be released into the environment gradually and cause a new environmental risk, and this risk is being taken seriously .
The release behaviors of heavy metals from cements and cementitious materials, as well as the release mechanisms and influence factors, have been studied to evaluate the environmental risk [5-10]. Actually, the distribution and the specific species of heavy metals in cement products are crucial for evaluating the environmental pollution risk because these affect the release behaviors of heavy metals greatly.
Most pieces of research previously conducted were focused on the distribution and the specific species of heavy metals in cement-based solidified/stabilized wastes [11-13]. Jing et al. have analyzed the arsenic species and components in cement-based solidified/stabilized wastes [14, 15]. Some studies revealed that the immobilization of arsenic with cement and lime is generally attributed to the formation of insoluble calcium arsenic compounds, such as CaHAs[O.sub.3] for arsenite containing wastes  and [Ca.sub.3][(As[O.sub.4]).sub.2] for S/S treated As(V)-bearing samples [17,18].
Although the distribution and the specific species of heavy metals in cement-based solidified/stabilized wastes were conducted, the study on the coprocessing cement product was limited. As the physical and chemical properties will be changed during calcination processes, the distribution and the specific species of heavy metals in the coprocessing cement product will be different from that in cement-based solidified/stabilized wastes . Therefore, it is essential to study the distribution and the specific species of heavy metals in the cement product from cement kiln coprocessing of wastes.
In this paper, a microscale investigation of arsenic in cement clinker and paste made with cement from simulated coprocessing wastes using cement kiln was conducted. Electron probe microanalysis (EPMA) was used to determine the As distribution and its associations with cement mineral phases, while X-ray absorption near edge structure (XANES) spectroscopy was used to obtain detailed information on the As valence state and major compounds in the cement clinker and paste. This information will be useful for evaluating the environmental pollution risk.
2. Materials and Methods
2.1. Raw Material Characterization. Raw cement materials, including limestone, clay, and iron powder, were obtained from a local cement plant, and their chemical compositions are listed in Table 1. The As contents in the raw materials, the amount of chemical reagents added in the experiment, and their corresponding ratios for cement production, which were calculated based on the arsenic content, are listed in Table 2.
2.2. Sample Preparation. [Na.sub.3]As[O.sub.4] x 12[H.sub.2]O was evenly mixed with the cement raw materials in accordance with the ratios listed in Table 2. A mass fraction of 1% distilled water was added to the mixture. After stirring regularly, disk samples (08O mm x 15 mm thick) were prepared. The disks were oven dried at 105[degrees]C and then calcined at 1450[degrees]C for 1h. Finally, the disks were rapidly cooled to room temperature in air. A portion of the clinkers were taken out and stored for XANES analysis.
A mass fraction of 5% gypsum was added to the remaining clinkers. Then the mixture was ground to fine cement consisting of particles with specific surface area of 310 [m.sup.2]/kg. Later, cement paste test pieces (20 x 20 x 10 mm) were made at a water to cement ratio of 0.3. They were first cured at 20[degrees] C and 96% relative humidity for 24 hour and then demolded. Finally, they were cured at (20 [+ or -] 2)[degrees]C and 95% relative humidity for 28 d prior to testing. Some of the cured cement test pieces were crushed in a jaw crusher until 95% of the sample was <125 [micro]m in size for XANES analysis.
2.3. Electron Probe Microanalysis. The remaining cement paste test pieces were placed in an oven at 60[degrees]C for 1-2 h. Once dry, the sample was soaked in epoxide-resin glue, and the temperature was increased to 50-60[degrees]C so that the epoxide-resin glue filled the spaces within the sample. Then the sample was placed in a vessel under a low vacuum to remove any air and cured in an oven at 60[degrees] C for 4 h. A diamond saw was used to cut smaller samples from the original sample, and then these cut samples were ground and polished for analysis by EPMA.
The microstructures were identified with the help of energy-dispersive X-ray spectroscopy (EDS, Oxford ISIS300), which is used to determine elemental composition. A JEOL JXA8800R EPMA analyzer was also used. The voltage employed was 15 keV, and the electron beam current was 2 x [10.sup.-8] A. BSE images and X-ray images (elemental distribution images) were acquired. National EPMA oxides and silicate standard samples were used.
The overall features of the cement mineral phase were first observed with the low power lens (scale of 200 [micro]m), and then typical mineral phases were transferred to the middle lens (scale of 50-100 [micro]m) for EPMA surface, line, and point analyses. Some mineral phases with fine particles were transferred to the high power lens (scale of 20 [micro]m) for these analyses.
2.4. XANES Measurements. Arsenic K-edge XANES spectra were collected at the Beijing Synchrotron Radiation Facility (BSRF). The typical energy of the storage ring was 2.5 GeV with the current decreasing from 250 to 160 mA during runs. [Mg.sub.3][(As[O.sub.4]).sub.2], [Ca.sub.3][(As[O.sub.4]).sub.2], [Na.sub.2]HAs[O.sub.4], [Na.sub.3]As[O.sub.4], and NaAs[O.sub.2] were recorded as standards in transmission mode (TM). Two samples, clinker and cement paste, were measured in fluorescence mode (FM). All standards were ground to fine grains and pressed to form wafers (01mm). Data analyses of the experimental XANES spectra were performed with FEFF8.0 .
3. Results and Discussion
3.1. Distribution and Association with Specific Mineral Phases. The elemental distribution image of As obtained with EPMA using the low-power lens is shown in Figure 1. Bright areas corresponding to high concentrations of As were very small and could not be distinguished easily. What also can be found is that the As is generally distributed throughout the cement paste.
BSE-imaging allows minerals of different compositions to be identified. Figure 2(a) shows a typical calcium silicate hydrates (C-S-H) gel feature. The elemental distribution map (Figure 2(b)) showed that the arsenic content was slightly associated with the C-S-H gels. Line analysis (Figure 3) of other typical C-S-H gel features confirmed this correlation.
Figure 4(a) shows the BSE image of a typical portlandite (CH crystal), and Figure 4(b) is the X-ray intensity curve along the line in Figure 4(a). This indicates that the arsenic content in the CH crystal is very low. The EDS analyses (Table 3) of random spots on the CH crystal confirmed this.
The EDS analyses (Table 4) of random spots on the intermediate phases, including calcium aluminates and calcium ferrites, indicated that their arsenic content was low.
A tentative explanation for the weak associations of arsenic with cement mineral phases is that most arsenic forms some arsenates dispersed on the surfaces of hydrates. These arsenates were mostly not incorporated into the hydrates in the calcination and hydration processes, and they became independent mineral phases adhered on the surfaces of hydrates. The association of arsenic with C-S-H phase maybe due to the high binding ability to arsenic compounds of C-S-H gels.
3.2. Specific Species of Arsenic. Arsenic K-edge XANES spectra of the samples and two standards are shown in Figure 5. The initial sharp peak in the XANES spectra arises from a transition of the excited photoelectron from the 1s level to vacant 4p levels. Huffman et al.  found that the energy of the s-p peak increased along with the valence state of the arsenic. Manning et al. [22, 23] indicated that the excitation energy for As(III) was well separated from that of As(V) by about 4 eV. In the present study, the peak energies for the cement paste and clinker were the same as that of sodium arsenate, in which the arsenic has a valence state of +5, and higher than that of sodium arsenite, in which the arsenic has a valence state of +3. This indicates that the arsenic in the cement paste and clinker has a valence state of +5.
The spectra of cement paste and clinker showed similar general trends. However, there were some interesting differences. For example, the s-p peak for the clinker was obviously more intense and narrower than that for the cement paste (Figure 5). Additionally, some secondary structures were visible from 11880-11900 eV for the clinker, but not evident for the cement paste. This suggests that the arsenic compounds in the clinker are crystalline.
Using the spectra of standards, LCF has been successfully applied to identify and quantify the main components of cement-immobilized materials . In this work, LCF was performed on the XANES data, and the fitting range was 144 eV around the absorption edge (about 11846-11990 eV). The fitting results are shown in Figure 6.
The main component in the cement paste was [Mg.sub.3][(As[O.sub.4]).sub.2] with a mass fraction of 55%. The other major components were [Na.sub.2]HAs[O.sub.4] and [Ca.sub.3][(As[O.sub.4]).sub.2] with mass fractions of 25% and 19.4%, respectively. By contrast, the content of [Na.sub.3]As[O.sub.4], which was the initial chemical added during production of the cement sample, was very low in the final product. Because [Mg.sub.3][(As[O.sub.4]).sub.2] and [Ca.sub.3][(As[O.sub.4]).sub.2] are stable compounds, most of the arsenic present in coprocessed cement can be immobilized.
Most of the arsenic in cement clinker and paste was present as more stable compounds, such as [Mg.sub.3][(As[O.sub.4]).sub.2] and [Ca.sub.3][(As[O.sub.4]).sub.2], which is formed in the cement production process.
Arsenic compounds in the clinker were similar to those in the cement paste, but they were crystalline instead of amorphous. This indicates that these compounds are mainly generated in the calcination process, and the hydration reaction contributes little to their formation. These stable compounds result in the immobilization of arsenic in co-processed products.
Arsenic compounds mainly disperse on the surfaces of the hydrates, only the C-S-H phase contained arsenic among the cement mineral phases, which may be due to the high binding ability to arsenic compounds of C-S-H gels.
The authors thank the staff of beamline 1W1B at the Beijing Synchrotron Radiation Facility (BSRF) and of beamline 14W1 at Shanghai Synchrotron Radiation Facility (SSRF). This research was supported by the National Natural Science Foundation of China (51178439).
 E. Mokrzycki, A. Uliasz-Bocheiiczyk, and M. Sarna, "Use of alternative fuels in the Polish cement industry" Applied Energy, vol. 74, no. 1-2, pp. 101-111, 2003.
 X. M. Zhu, J. G. Liu, and Q. F. Huang, "The application and existing problems of co-processing technology of hazardous waste in cement kiln" China Cement, vol. 4, pp. 45-49, 2006 (Chinese).
 D. H. Yan, K. H. Karstensen, Q. F. Huang, Q. Wang, and M. Cai, "Coprocessing of industrial and hazardous wastes in cement kilns: a review of current status and future needs in China" Environmental Engineering Science, vol. 27, no. 1, pp. 37-45,2010.
 Q. F. Huang, Y. F. Yang, and Q. Wang, "Potential for serious environmental threats from uncontrolled co-processing of wastes in cement kilns" Environmental Science and Technology, vol. 46, no. 24, pp. 13031-13032, 2012.
 D. S. Kosson, H. A. van der Sloot, F. Sanchez, and A. C. Garrabrants, "An integrated framework for evaluating leaching in waste management and utilization of secondary materials," Environmental Engineering Science, vol. 19, no. 3, pp. 159-204, 2002.
 D. S. Kosson, H. A. van der Sloot, and T. T. Eighmy, "An approach for estimation of contaminant release during utilization and disposal of municipal waste combustion residues," Journal of Hazardous Materials, vol. 47, no. 1-3, pp. 43-75,1996.
 H. A. van der Sloot, "Characterization of the leaching behaviour of concrete mortars and of cement-stabilized wastes with different waste loading for long term environmental assessment," Waste Management, vol. 22, no. 2, pp. 181-186, 2002.
 F. Sanchez, C. Gervais, A. C. Garrabrants, R. Barna, and D. S. Kosson, "Leaching of inorganic contaminants from cement-based waste materials as a result of carbonation during intermittent wetting" Waste Management, vol. 22, no. 2, pp. 249-260, 2002.
 A. C. Garrabrants, F. Sanchez, and D. S. Kosson, "Changes in constituent equilibrium leaching and pore water characteristics of a Portland cement mortar as a result of carbonation" Waste Management, vol. 24, no. 1, pp. 19-36, 2004.
 Y. F. Yang, Y. Yang, Q. F. Wang, and Q. Huang, "Release of heavy metals from concrete made with cement from cement kiln co-processing of hazardous wastes in pavement scenarios" Environmental Engineering Science, vol. 28, no. 1, pp. 35-42, 2011.
 Q. Y. Chen, M. Tyrer, C. D. Hills, X. M. Yang, and P. Carey, "Immobilisation of heavy metal in cement-based solidification/stabilisation: a review" Waste Management, vol. 29, no. 1, pp. 390-403, 2009.
 M. Pomies, N. Lequeux, and P Boch, "Speciation of cadmium in cement--part I. [Cd.sup.2+] uptake by C-S-H" Cement and Concrete Research, vol. 31, no. 4, pp. 563-569, 2001.
 M. P Pomies, N. Lequeux, and P Boch, "Speciation of cadmium in cement--part II. [C.sub.3]S hydration with [Cd.sup.2+] solution" Cement and Concrete Research, vol. 31, no. 4, pp. 571-576, 2001.
 C. Jing, G. P. Korfiatis, and X. Meng, "Immobilization mechanisms of arsenate in iron hydroxide sludge stabilized with cement" Environmental Science and Technology, vol. 37, no. 21, pp. 5050-5056, 2003.
 C. Jing, S. Liu, and X. Meng, "Arsenic leachability and speciation in cement immobilized water treatment sludge," Chemosphere, vol. 59, no. 9, pp. 1241-1247, 2005.
 V. Dutre and C. Vandecasteele, "Immobilization mechanism of arsenic in waste solidified using cement and lime," Environmental Science and Technology, vol. 32, no. 18, pp. 2782-2787,1998.
 M. Y. A. Mollah, F. Lu, and D. L. Cocke, "An X-ray diffraction (XRD) and Fourier transform infrared spectroscopic (FT-IR) characterization of the speciation of arsenic (V) in Portland cement type-V" Science of the Total Environment, vol. 224, no. 1-3, pp. 57-68,1998.
 C. Vandecasteele, V Dutre, D. Geysen, and G. Wauters, "Solidification/stabilisation of arsenic bearing fly ash from the metallurgical industry. Immobilisation mechanism of arsenic," Waste Management, vol. 22, no. 2, pp. 143-146, 2002.
 J. Zhang, J. Liu, C. Li, Y. Jin, Y. Nie, and J. Li, "Comparison of the fixation effects of heavy metals by cement rotary kiln co-processing and cement based solidification/stabilization," Journal of Hazardous Materials, vol. 165, no. 1-3, pp. 1179-1185, 2009.
 A. L. Ankudinov, B. Ravel, J. J. Rehr, and S. D. Conradson, "Real-space multiple-scattering calculation and interpretation of X-ray-absorption near-edge structure," Physical Review B, vol. 58, no. 12, pp. 7565-7576,1998.
 G. P Huffman, F. E. Huggins, N. Shah, and J. Zhao, "Speciation of arsenic and chromium in coal and combustion ash by XAFS spectroscopy," Fuel Processing Technology, vol. 39, no. 1-3, pp. 47-62,1994.
 B. A. Manning, S. E. Fendorf, and S. Goldberg, "Surface structures and stability of arsenic(III) on goethite: spectroscopic evidence for inner-sphere complexes," Environmental Science and Technology, vol. 32, no. 16, pp. 2383-2388,1998.
 B. A. Manning, S. E. Fendorf, B. Bostick, and D. L. Suarez, "Arsenic(III) oxidation and arsenic(V) adsorption reactions on synthetic birnessite," Environmental Science and Technology, vol. 36, no. 5, pp. 976-981, 2002.
Yufei Yang, (1) Jingchuan Xue, (2) and Qifei Huang (1)
(1) State Key Laboratory of Environmental Criteria and Risk Assessment, Chinese Research Academy of Environmental Science, Beijing 100012, China
(2) Wadsworth Center, New York State Department of Health, and Department of Environmental Health Sciences, School of Public Health, State University of New York at Albany, Empire State Plaza, P.O. Box 509, Albany, NY 12210-0509, USA
Correspondence should be addressed to Qifei Huang; firstname.lastname@example.org
Received 9 July 2013; Accepted 15 September 2013
Academic Editors: S. R. Kanel and R. A. Smith
TABLE 1: Chemical composition of raw materials (%). Items Si[O.sub.2] [Fe.sub.2] [Al.sub.2] [O.sub.3] [O.sub.3] Limestone 0.18 0.04 0.04 Clay 62.14 9.10 16.17 Ion powder 34.98 50.56 4.95 Items CaO MgO LOSS Limestone 55.64 0.05 43.40 Clay 1.63 0 7.30 Ion powder 1.34 0.84 4.52 TABLE 2: Design and materials in experiment. Items As Ni content in the raw 81.6 material (1)/(mg x [kg.sup.-1]) Chemical reagents added [Na.sub.3]As[O.sub.4] x 12[H.sub.2]O Adding ratio (1)/% 0.3 Adding amount in the raw 17 material (1)/g x [kg.sup.-1] 1 Calculated by w. TABLA 3: EPMA point analysis data of CH crystal in cement paste. Number Element content (%) Al Si Ca Fe As 1 0.09 0.85 60.47 0.65 0 2 0.05 0.79 56.78 0.66 0.03 3 0.15 1.07 57.69 0.45 0.28 4 0 2.56 36.32 0.62 0.52 5 0.20 2.71 37.78 0.68 0.42 6 0.13 1.16 54.44 0.79 0 7 0.27 1.49 57.05 0.66 0 8 0.27 1.25 56.79 0.59 0 9 0.43 3.06 54.23 0.70 0 TABLE 4: EPMA point analysis data of middle phases containing Fe, Al in cement paste. Number Element content (%) Al Si Ca Fe As 1 17.21 6.12 50.80 15.16 0 2 19.70 4.39 50.19 16.69 0 3 20.27 4.06 48.71 17.08 0 4 20.77 4.15 47.93 16.82 0 5 19.28 4.03 50.23 17.96 0 6 21.70 4.18 48.05 17.42 0 7 20.54 4.21 50.54 16.60 0 8 19.35 4.06 51.66 15.25 0 9 21.39 4.36 47.57 16.97 0 10 20.91 4.30 47.39 15.14 0
|Printer friendly Cite/link Email Feedback|
|Title Annotation:||Research Article|
|Author:||Yang, Yufei; Xue, Jingchuan; Huang, Qifei|
|Publication:||The Scientific World Journal|
|Date:||Jan 1, 2013|
|Previous Article:||Comparative analysis and systematic mapping of the labial sensilla in the nepomorpha (Heteroptera: Insecta).|
|Next Article:||Nexfin noninvasive continuous hemodynamic monitoring: validation against continuous pulse contour and intermittent transpulmonary thermodilution...|